Hindawi Publishing CorporationISRN CorrosionVolume 2013, Article ID 905942, 7 pageshttp://dx.doi.org/10.1155/2013/905942
Research ArticleMorphology Characterisation of Pitting Corrosion on SensitizedAustenitic Stainless Steel by Digital Image Analysis
R. B. Ribeiro,1 J. W. J. Silva,1,2 L. R. O. Hein,2 M. C. Pereira,2
E. N. Codaro,2 and N. T. Matias1
1 Faculdades Integradas Teresa DAvila, FATEA-Rede salesianas, Avenida Peixoto de Castro 539, Vila Celeste,12606-580 Lorena, SP, Brazil
2 Universidade Estadual Paulista, UNESP-Campus de Guaratingueta, Avenida Ariberto Pereira da Cunha 333,Pedregulho, 12.516-410 Guaratingueta, SP, Brazil
Correspondence should be addressed to J. W. J. Silva; firstname.lastname@example.org
Received 30 May 2013; Accepted 14 July 2013
Academic Editors: G. Bereket, S. Caporali, and R. Salghi
Copyright 2013 R. B. Ribeiro et al. This is an open access article distributed under the Creative Commons Attribution License,which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Pit morphology on sensitized 310S stainless steel has been studied using an image processing method based on reflected lightmicroscopy. Salt Spray (fog) test has been used to induce the pitting corrosion. Morphological pits characters do not dependon sensitization heat treatments applied here. Nucleation rates and growth may be associated with quantity and distribution ofchromium carbides. This being so, condition I (heating up to 1065C during 1 h and air cooling) and condition II (heating up to1065C during 1 h and air cooling followed by reheating up to 670C during 5 h and again air cooling) are the most susceptible topitting, in particular the first one. In these two conditions, pits are nucleated in grains and in grain boundaries, while in conditionIII (heating up to 1065C during 1 h and air cooling followed by reheating up to 620C during 24 h and again air cooling), pits arepreferentially nucleated in boundaries of small grains. Thence, pits usually grow more rapidly in depth than in width, being ableto occur partial or total grains separation. Pits are mainly hemispherical, near-hemispherical, near-conical, and near-cylindricalwithout significant geometric transition associated with an increasing exposure period.
Austenitic stainless steel is selected for corrosion resistanceto the atmosphere and a vast variety of chemical products.This resistance is related to the formation of a thin andadherent oxides layer (mainly Cr
2O3), which protects the
surface against aggressive environments. The most commonaustenitic steel is iron-chromium-nickel alloys and theyare widely known as the 300 series. These alloys usuallycontain between 16 and 30wt% chromium, 8 to 20% nickel,and 0.03 to 0.1% carbon. With increasing chromium andnickel contents, this steel becomes increasingly resistant topitting corrosion. However, the higher concentrations ofthese alloying elements result in lower carbon solubility andcarbide segregation. Heat treatments, whether intentionalor accidental, may provoke carbide precipitation at grainboundaries, often by causing steel to become susceptibleto intergranular corrosion. In order to minimize carbide
precipitation and prevent to sensitization, austenitic steel isfrequently subjected to high-temperature solution treatment,commonly termed quench-annealing [1, 2]. Pitting corrosionis observed in austenitic steel exposed to aqueous mediacontaining chloride ions. This phenomenon almost alwaysstarts in anodicMnS inclusions and chromium-depleted zoneadjacent to cathodic M
23C6(M = Cr or Mo) precipitates,
and it progresses inwards in intergranular or transgranulardirection dependingmainly on the steelmicrostructure [2, 3].
Many studies have been focused on the pit initiationand propagation mechanisms of this steel in chloride media, but relatively a few authors have considered themorphologic characteristics of pitting corrosion. It should benoted that pit growth rate depends on potential distributioninside the pit, which is determined by pit shape, especiallyby their width/depth aspect ratio [11, 12]. For pits initiatedby electrochemical experiments, the pit depth or pit radiusdependence on the immersion time () may be expressed by
2 ISRN Corrosion
the equation ( ), where
is the induction period, > 0,
and 1/3 1 are empirical constants which dependon chloride concentration, pits shape, and experimentalconditions inherent of electrochemical methods. Pits areusually modelled as having cylindrical, hemispherical, orconical shapes, but in practice, they have a tendency toassume an irregular or not well-defined geometry associatedwith increasing size . Therefore, equations, developedwith these assumptions about shape, must be considered asonly rough approximations.
In this study, a method based on image analysis has beenused for themorphology characterization of pitting corrosionon sensitized 310S steel. For this purpose, pits have beeninitiated by Salt Spray exposure, and their temporal evolutionhas been examined by reflected light microscopy.
2. Materials and Methods
As-received, 310S plates  have been submitted to threesolution heat treatment routines: heating up to 1065C during1 h and air cooling (condition I); heating up to 1065C during1 h and air cooling followed by reheating up to 670C during5 h and again air cooling (condition II); heating up to 1065Cduring 1 h and air cooling followed by reheating up to 620Cduring 24 h and again air cooling (condition III). The mainpurpose for annealing has been to produce a recrystallizedmicrostructure with a uniform grain size and for dissolvingdetrimental chromium carbide precipitates. Then, a slowcooling or reheating within the range 550800C will leadto the rejection of carbon from solution, usually as thechromium-rich carbide, even when the carbon content of thesteel is very low (
ISRN Corrosion 3
Figure 2: LM micrographs of 310S sensitized before Salt Spray test: (a) condition I, (b) condition II, and (c) condition III.
0 1 2 3 4 5 6 7 8 9 10 11(keV)
Full scale 14458 cts Cursor: 8.809 keV (129 cts)
0 1 2 3 4 5 6 7 8 9 10 11(keV)
Full scale 8698 cts Cursor: 7.824 keV (158 cts)
Figure 3: EDS semiquantitative analysis upon the 310S in condition II: (a) grain and (b) precipitate in grain boundary.
4 ISRN Corrosion
Table 1: Variation of pitting corrosion parameters measured on exposed surfaces.
Parameter Heat treatment Exposure period (h)48 120 168 216 312
Pit density (mm2)I 15.98 28.02 39.76 200.09 378.06II 19.03 25.15 34.12 34.16 40.20III 9.02 10.45 15.34 14.09 19.99
Corroded area (%)I 0.08 0.20 0.44 0.50 2.40II 0.04 0.10 0.55 0.90 1.89III 0.09 0.08 0.80 1.20 3.90
Area at mouth (m2)I 10.09 11.98 12.65 12.32 13.07II 8.87 9.67 20.14 25.08 29.76III 13.45 15.11 25.23 26.23 35.28
Table 2: Classification and distribution of pits percentages.
Pit geometry Heat treatment Exposure period (h)48 120 168 216 312
Irregular (%)I 6.41 0.67 0.66 4.19 0.00II 1.71 7.43 3.75 5.36 6.67III 0.00 3.17 15.87 6.44 12.30
Conical (%)I 1.28 4.67 1.32 2.80 1.23II 0.00 6.93 5.00 2.68 1.02III 0.00 2.08 2.59 13.30 6.56
Transition region A (%)I 7.70 54.66 14.47 26.57 3.47II 20.50 24.36 24.16 27.68 30.45III 18.14 27.09 26.98 61.80 39.33
Hemispherical (%)I 19.23 29.33 28.29 17.48 20.99II 23.08 18.80 36.71 41.96 42.56III 24.29 28.40 29.16 15.88 24.60
Transition region B (%)I 65.38 10.67 55.26 48.96 74.31II 54.71 42.48 30.38 22.32 19.30III 57.57 39.26 25.40 2.58 17.21
Cylindrical (%)I 0.00 0.00 0.00 0.00 0.00II 0.00 0.00 0.00 0.00 0.00III 0.00 0.00 0.00 0.00 0.00
behaviour, in distribution, and in morphology of pits atmaterial as received and treated.
After corrosion test, surfaces have revealed pits of differ-ent shapes and sizes. Table 1 permits to compare statisticalparameters measured on exposed surfaces. For all heat treat-ment conditions, low values of corroded areas suggest thereis a low probability of pit superposition during the exposureperiod. Thus, the temporal variation in pit density and pitarea may be directly related to the rates of pit nucleation andtwo-dimensional growth, respectively. This way, nucleationrate has remained approximately constant for conditions IIand III, and it has increased for condition I. In this lastcondition, the pits growth is slower. These facts are mainlyrelated with a number of anodic sites and anodic/cathodicarea ratio variation during exposure period.
Conditions I and II, pits are nucleated in grains andgrain boundaries, while in condition III, pits are preferentially
nucleated in boundaries of small grains. Generally, carbidesare too fine to be resolved by reflected light microscopebut are indirectly revealed by deep etching of affected grainboundaries (Figure 4(c)). Pits classification and distributionhave been determined from cross-section images. Table 2indicates that for all conditions: (i) the hemispherical, near-hemispherical, near-conical, and near-cylindrical pits repre-sent more than 80% of the pit population; (ii) they appear notto undergo geometric transition associatedwith an increasingexposure period; (iii) pits with regular geometry representless than 45%of pit population; (iv) cylindrical pits are absent.This geometry distribution may be attribu